Dark dimer mode excitation and strong coupling with a nanorod dipole
We theoretically investigate dark dimer mode excitation and strong coupling with a nanorod dipole. Efficient excitation of a dark mode in a gold (Au) nanorod dimer using an electric dipole can be achieved by an optimal overlap between the dipole moment and dark modal field. By replacing the dipole emitter with an Au nanorod, a plane wave excited dipole mode in the nanorod can be effectively coupled to the dark dimer mode through near-field interaction. At a 10-nm separation of the nanorod and the dimer, plasmonic interaction between dipole-dark modes enters the strong coupling regime with a Rabi-like splitting of 219.2 meV, which is further evidenced by the anticrossing feature and Rabi-like oscillation of electromagnetic energy of the coupled modes. Our results propose an efficient approach to far-field activating dark modes in coupled nanorod dimers and exchanging plasmonic excitations at nanoscale, which may open new opportunities for nanoplasmonic applications such as nanolasers or nanosensors.
基金项目：National Natural Science Foundation of China (NSFC)10.13039/501100001809 (11527901, 61475136, 61635009); Fundamental Research Funds for the Central Universities; China Postdoctoral Science Foundation10.13039/501100002858 (2018M632454, BX201700207).
Ning Zhou：State Key Laboratory of Modern Optical Instrumentation, College of Optical Science and Engineering, Zhejiang University, Hangzhou 310027, China
Zhangxing Shi：State Key Laboratory of Modern Optical Instrumentation, College of Optical Science and Engineering, Zhejiang University, Hangzhou 310027, China
Xin Guo：State Key Laboratory of Modern Optical Instrumentation, College of Optical Science and Engineering, Zhejiang University, Hangzhou 310027, China
Limin Tong：State Key Laboratory of Modern Optical Instrumentation, College of Optical Science and Engineering, Zhejiang University, Hangzhou 310027, ChinaCollaborative Innovation Center of Extreme Optics, Shanxi University, Taiyuan 030006, Chinae-mail: firstname.lastname@example.org
【1】W. L. Barnes, A. Dereux, and T. W. Ebbesen, “Surface plasmon subwavelength optics,” Nature 424 , 824–830 (2003).
【2】Z. Wang, X. Meng, A. V. Kildishev, A. Boltasseva, and V. M. Shalaev, “Nanolasers enabled by metallic nanoparticles: from spasers to random lasers,” Laser Photon. Rev. 11 , 1700212 (2017).
【3】J. N. Anker, W. P. Hall, O. Lyandres, N. C. Shah, J. Zhao, and R. P. Van Duyne, “Biosensing with plasmonic nanosensors,” Nat. Mater. 7 , 442–453 (2008).
【4】H. Shen, R. Y. Chou, Y. Y. Hui, Y. He, Y. Cheng, H.-C. Chang, L. Tong, Q. Gong, and G. Lu, “Directional fluorescence emission from a compact plasmonic-diamond hybrid nanostructure,” Laser Photon. Rev. 10 , 647–655 (2016).
【5】R. Chikkaraddy, B. de Nijs, F. Benz, S. J. Barrow, O. A. Scherman, E. Rosta, A. Demetriadou, P. Fox, O. Hess, and J. J. Baumberg, “Single-molecule strong coupling at room temperature in plasmonic nanocavities,” Nature 535 , 127–130 (2016).
【6】H. Wang, D. W. Brandl, P. Nordlander, and N. J. Halas, “Plasmonic nanostructures: artificial molecules,” Acc. Chem. Res. 40 , 53–62 (2007).
【7】N. Papasimakis, V. A. Fedotov, N. I. Zheludev, and S. L. Prosvirnin, “Metamaterial analog of electromagnetically induced transparency,” Phys. Rev. Lett. 101 , 253903 (2008).
【8】R. Guo, M. Decker, F. Setzpfandt, I. Staude, D. N. Neshev, and Y. S. Kivshar, “Plasmonic Fano nanoantennas for on-chip separation of wavelength-encoded optical signals,” Nano Lett. 15 , 3324–3328 (2015).
【9】C. Wu, A. B. Khanikaev, R. Adato, N. Arju, A. A. Yanik, H. Altug, and G. Shvets, “Fano-resonant asymmetric metamaterials for ultrasensitive spectroscopy and identification of molecular monolayers,” Nat. Mater. 11 , 69–75 (2011).
【10】P. Nordlander, C. Oubre, E. Prodan, K. Li, and M. I. Stockman, “Plasmon hybridization in nanoparticle dimers,” Nano Lett. 4 , 899–903 (2004).
【11】H. Xu, J. Aizpurua, M. K?ll, and P. Apell, “Electromagnetic contributions to single-molecule sensitivity in surface-enhanced Raman scattering,” Phys. Rev. E 62 , 4318–4324 (2000).
【12】H. Aouani, M. Rahmani, M. Navarro-Cia, and S. A. Maier, “Third-harmonic-upconversion enhancement from a single semiconductor nanoparticle coupled to a plasmonic antenna,” Nat. Nanotechnol. 9 , 290–294 (2014).
【13】A. F. Koenderink, “Single-photon nanoantennas,” ACS Photon. 4 , 710–722 (2017).
【14】A. M. Michaels, J. Jiang, and L. Brus, “Ag nanocrystal junctions as the site for surface-enhanced Raman scattering of single rhodamine 6G molecules,” J. Phys. Chem. B 104 , 11965–11971 (2000).
【15】K. D. Osberg, N. Harris, T. Ozel, J. C. Ku, G. C. Schatz, and C. A. Mirkin, “Systematic study of antibonding modes in gold nanorod dimers and trimers,” Nano Lett. 14 , 6949–6954 (2014).
【16】S. Zhang, L. Chen, Y. Huang, and H. Xu, “Reduced linewidth multipolar plasmon resonances in metal nanorods and related applications,” Nanoscale 5 , 6985–6991 (2013).
【17】D. E. Gomez, Z. Q. Teo, M. Altissimo, T. J. Davis, S. Earl, and A. Roberts, “The dark side of plasmonics,” Nano Lett. 13 , 3722–3728 (2013).
【18】M. Ramezani, A. Halpin, A. I. Fernández-Domínguez, J. Feist, S. R.-K. Rodriguez, F. J. Garcia-Vidal, and J. Gómez Rivas, “Plasmon-exciton-polariton lasing,” Optica 4 , 31–37 (2017).
【19】T. K. Hakala, H. T. Rekola, A. I. Vakevainen, J. P. Martikainen, M. Necada, A. J. Moilanen, and P. Torma, “Lasing in dark and bright modes of a finite-sized plasmonic lattice,” Nat. Commun. 8 , 13687 (2017).
【20】D. Zheng, S. Zhang, Q. Deng, M. Kang, P. Nordlander, and H. Xu, “Manipulating coherent plasmon-exciton interaction in a single silver nanorod on monolayer WSe2,” Nano Lett. 17 , 3809–3814 (2017).
【21】B. Yun, G. Hu, J. Cong, and Y. Cui, “Fano resonances induced by strong interactions between dipole and multipole plasmons in T-shaped nanorod dimer,” Plasmonics 9 , 691–698 (2014).
【22】Z. J. Yang, Z. S. Zhang, L. H. Zhang, Q. Q. Li, Z. H. Hao, and Q. Q. Wang, “Fano resonances in dipole-quadrupole plasmon coupling nanorod dimers,” Opt. Lett. 36 , 1542–1544 (2011).
【23】P. K. Jha, M. Mrejen, J. Kim, C. Wu, X. Yin, Y. Wang, and X. Zhang, “Interacting dark resonances with plasmonic meta-molecules,” Appl. Phys. Lett. 105 , 111109 (2014).
【24】N. Liu, L. Langguth, T. Weiss, J. Kastel, M. Fleischhauer, T. Pfau, and H. Giessen, “Plasmonic analogue of electromagnetically induced transparency at the Drude damping limit,” Nat. Mater. 8 , 758–762 (2009).
【25】Z. J. Yang, Z. H. Hao, H. Q. Lin, and Q. Q. Wang, “Plasmonic Fano resonances in metallic nanorod complexes,” Nanoscale 6 , 4985–4997 (2014).
【26】C. J. Tang, P. Zhan, Z. S. Cao, J. Pan, Z. Chen, and Z. L. Wang, “Magnetic field enhancement at optical frequencies through diffraction coupling of magnetic plasmon resonances in metamaterials,” Phys. Rev. B 83 , 041402 (2011).
【27】R. Ameling, and H. Giessen, “Cavity plasmonics: large normal mode splitting of electric and magnetic particle plasmons induced by a photonic microcavity,” Nano Lett. 10 , 4394–4398 (2010).
【28】Z. Xi, Y. Lu, W. Yu, P. Yao, P. Wang, and H. Ming, “Strong coupling between plasmonic Fabry–Pérot cavity mode and magnetic plasmon,” Opt. Lett. 38 , 1591–1593 (2013).
【29】R. Ameling, D. Dregely, and H. Giessen, “Strong coupling of localized and surface plasmons to microcavity modes,” Opt. Lett. 36 , 2218–2220 (2011).
【30】P. Wang, Y. Wang, Z. Yang, X. Guo, X. Lin, X. C. Yu, Y. F. Xiao, W. Fang, L. Zhang, G. Lu, Q. Gong, and L. Tong, “Single-band 2-nm-line-width plasmon resonance in a strongly coupled Au nanorod,” Nano Lett. 15 , 7581–7586 (2015).
【31】D. Y. Lu, H. Liu, T. Li, S. M. Wang, F. M. Wang, S. N. Zhu, and X. Zhang, “Creation of a magnetic plasmon polariton through strong coupling between an artificial magnetic atom and the defect state in a defective multilayer microcavity,” Phys. Rev. B 77 , 214302 (2008).
【32】H. Chen, L. Shao, Q. Li, and J. Wang, “Gold nanorods and their plasmonic properties,” Chem. Soc. Rev. 42 , 2679–2724 (2013).
【33】P. B. Johnson, and R. W. Christy, “Optical constants of the noble metals,” Phys. Rev. B 6 , 4370–4379 (1972).
【34】M. Liu, T. W. Lee, S. K. Gray, P. Guyot-Sionnest, and M. Pelton, “Excitation of dark plasmons in metal nanoparticles by a localized emitter,” Phys. Rev. Lett. 102 , 107401 (2009).
【35】S. C. Yang, H. Kobori, C. L. He, M. H. Lin, H. Y. Chen, C. Li, M. Kanehara, T. Teranishi, and S. Gwo, “Plasmon hybridization in individual gold nanocrystal dimers: direct observation of bright and dark modes,” Nano Lett. 10 , 632–637 (2010).
【36】D. G. Baranov, M. Wers?ll, J. Cuadra, T. J. Antosiewicz, and T. Shegai, “Novel nanostructures and materials for strong light-matter interactions,” ACS Photon. 5 , 24–42 (2017).
【37】W. Chen, S. Zhang, Q. Deng, and H. Xu, “Probing of sub-picometer vertical differential resolutions using cavity plasmons,” Nat. Commun. 9 , 801 (2018).
【38】H. Harutyunyan, G. Volpe, R. Quidant, and L. Novotny, “Enhancing the nonlinear optical response using multifrequency gold-nanowire antennas,” Phys. Rev. Lett. 108 , 217403 (2012).
【39】M. Celebrano, X. Wu, M. Baselli, S. Grossmann, P. Biagioni, A. Locatelli, C. De Angelis, G. Cerullo, R. Osellame, B. Hecht, L. Duo, F. Ciccacci, and M. Finazzi, “Mode matching in multiresonant plasmonic nanoantennas for enhanced second harmonic generation,” Nat. Nanotechnol. 10 , 412–417 (2015).
【40】A. V. Akimov, A. Mukherjee, C. L. Yu, D. E. Chang, A. S. Zibrov, P. R. Hemmer, H. Park, and M. D. Lukin, “Generation of single optical plasmons in metallic nanowires coupled to quantum dots,” Nature 450 , 402–406 (2007).
Yixiao Gao, Ning Zhou, Zhangxing Shi, Xin Guo, and Limin Tong, "Dark dimer mode excitation and strong coupling with a nanorod dipole," Photonics Research 6(9), 887-892 (2018)